Chem. Mater. 1994, 6, 2005-2007 2005 Structure of Sr3Sc(B03>3 Paul D. Thompson and Douglas A. Keszler* Department of Chemistry and Center for Advanced Materials Research, Oregon State University, Gilbert Hall 153, Corvallis, Oregon 97331-4003 Downloaded via UNIV OF CAMBRIDGE on September 3, 2019 at 14:25:20 (UTC). See https://pubs.acs.org/sharingguidelines for options on how to legitimately share published articles. Received April 20, 1994. Revised Manuscript Received August 29, 1994® The structure of the compound Sr3Sc(BC>3)3 is described. Crystal data: FW = 484.24 amu, R3 (No. 148), hexagonal axes, a = 12.135(1), c = 9.184(1) A, V= 1171.3(2) A3, Z = 6, Mo Ka = 0.022 for 725 (A = 0.710 69 A), fi = 206.38 cm"* 1, F(000) = 1332, T = 296 K, R = 0.018, averaged reflections. The structure exhibits chains comprised of Sc-centered O octahedra and BO3 triangles that are bridged by 9-coordinate Sr atoms. Each chain contains two crystallographically independent Sc atoms; the distorted octahedral environment about atom = Scl is compressed along the trigonal axis, Ol-Scl-Ol 85.20(7)°, while the environment about atom Sc2 is elongated along the same axis, 02-Sc2-02 = 92.28(7)°. These angles are consistent with the chemical inequivalence of the environments as determined by their associations with neighboring Sr atoms. Introduction Table 1. Crystal Data and Experimental Conditions for Sr3Sc(B03)3 This report is the first in a series detailing the crystal chemistry of borates derived from the general formula A3M(BC>3)3 and represented by the structural types of the parent compounds Sr3Sc(B03)3 and Ba3Sc(BC>3)3. As we have reported,1 derivatives of the Sr compound now comprise one of the larger structural families of solidstate oxide discovered to date. A detailed discussion of these derivatives is given in the third paper of this formula FW, Sr3Sc(B03)3 484.24 R3 12.135(1) 9.184(1) 1171.3(2) amu space group a, A c, A V, A3 z T of data collection, K Pealed, series. 6 296 4.12 g cm-3 radiation graphite monochromated Mo Ka tt(Ka) 0.710 69 A) ^ cm-1 206.38 transmission factors 0.932-1.089 Rint Rw(Fo) R(F0) for F02 0.032 0.022 0.018 = Here, following, we describe the structure of the compound Sr3Sc(B(>3)3, a material that exhibits potentially useful optical characteristics when doped with the ion Cr3+.2 In the ensuing papers we discuss the structure of the compound Ba3Sc(BC>3)3, the derivatives of both structural types, and the interrelationships between them. Zo(Fo2) Table 2. Atomic Parameters for SrsScfBOsh0 atom Experimental Section y z Be q 0.03998(2) 0.46988(2) 0.30855(2) 0 0 0 0 v2 0 0.4699(3) 0.1644(2) 0.3683(2) 0.2637(2) 0.0994(3) 0.3809(2) 0.1934(2) 0.1865(2) 0.636(9) 0.45(2) 0.46(2) 0.65(8) 0.79(6) 0.72(5) 0.81(6) X Sr Scl 0.1406(3) 0.0522(2) Sc2 Single crystals of the title compound were grown in a Pt crucible from a melt of composition 40 mol % SrO, 10 mol % SC2O3, 40 mol % B2O3, and 10 mol % Li20 that was cooled from 1313 to 773 K at 6 K/h. The crystals were isolated by treating the solidified melt with dilute HN03(aq). Unit-cell parameters were determined from least-squares refinement of 20 reflections in the range 17 < 29 < 35° that had been automatically centered on a Rigaku AFC6R diffractometer. A check of the Laue symmetry on the diffractometer revealed that the material crystallized in group 3. Crystal data and experimental conditions for the X-ray measurements are given in Table 1. Three standard reflections that were measured after each block of 200 data exhibited an overall average excursion of B 01 02 03 a Beq -0.1779(2) 0.0047(2) = (8jr2/3)SiSj[/ya,;*aj*araj. variables, and anisotropic displacement coefficients on each atom. The largest peak in the final difference electron density map corresponds to 1.3% of a Sr atom. Analysis of the residuals as a function of Miller indices and |F0| reveals no unusual trends. Final atomic parameters are listed in Table 2. Results and Discussion Calculations were performed on a wVAX-II computer with programs from the TEXSAN system of programs.3 Final leastsquares refinement on F„ included 725 averaged data, 51 A labeled drawing of the contents of the unit cell is given in Figure 1. The structure is simple and readily described as a collection of one-dimensional chains (Figure 2) extending along the c axis. Each chain contains Sc-centered distorted octahedra that are linked by triangular BO3 groups. Two nonequivalent Sc sites are present in each chain, and they alternate in their lodgments along the chain axis. The chains, packing * To whom correspondence should be addressed. Abstract published in Advance ACS Abstracts, October 15, 1994. (1) Schaffers, K. I.; Alekel III, T.; Thompson, P. D.; Cox, J. R.; Keszler, D. A. J. Am. Chem. Soc. 1990, 112, 7068. (2) Thompson. P. D.; Keszler, D. A. Chem. Mater. 1989, 1, 292. (3) TEXSAN: Single Crystal Structure Analysis Software, Version 5.0,1989. Molecular Structure Corporation, The Woodlands, TX 77381. ® 0897-4756/94/2806-2005$04.50/0 > © 1994 American Chemical Society 2006 Thompson and Keszler Chem. Mater., Vol. 6, No. 11, 1994 1. Sketch of the contents of the unit cell for the compound Sr3Sc(B03)3. Sr atoms are indicated as small lined circles, Sc atoms as small open circles, B atoms as small filled circles, and O atoms as large shaded circles, here and in all subsequent figures. Figure Table 3. Interatomic Sr-03 Sr-02 Sr-03 Sr-01 Sr-01 Sr-03 Sr-02 Sr-01 Sr-03 Sr-O(av) Scl-Ol Sc2-02 B-Ol B-02 B-03 B-O(av) Figure 2. Drawing of an individual chain containing Scl- and Sc2-centered distorted octahedra bridged by B03 groups. Distances (A) and Angles (deg) for Sr3Sc(B03)3 2.500(2) 2.524(2) 2.574(2) 2.714(2) 2.758(2) 2.760(2) 2.760(2) 2.765(2) 2.857(2) 01-Sr-02 Ol-Sr-Ol 02—Sr-03 02—Sr-03 Ol-Sr-02 02-Sr-03 Ol-Sr-02 Ol-Sr-02 51.20(6) 61.19(7) 70.12(5) 84.48(6) 94.50(6) 109.20(6) 125.40(6) 144.64(6) 01-Scl-01 02-Sc2-02 03-B-02 03-B-01 02-B-01 85.20(7) 92.28(7) 121.2(2) 119.9(2) 118.7(2) 2.6903) 2.077(2) 2.142(2) 1.388(3) 1.383(3) 1.364(3) 1.38(1) according to the rhombohedral centering conditions of the cell, are bridged by Sr atoms occupying 9-coordinate environments. Linkage of these Sr-centered polyhedra in all directions, however, mitigates the anisotropy to be expected from the chain description, affording instead a dense, pure three-dimensional structure. Selected interatomic distances and angles are listed in Table 3. Atoms Scl and Sc2 occupy distorted octahedral sites having S& (3) point-group symmetry. The Scl-Ol distance is 2.077(2) A and the Ol octahedron is slightly compressed along the trigonal axis, Ol Scl-Ol = 85.20(7)°. The Sc2-02 distance, 2.142(2) A, is longer and the 02 octahedron is now trigonally elongated, 02-Sc2-02 = 92.28(7)°. These interatomic distances and angles may be compared to the Sc-0 distance 2.120(2) A and the trigonal elongation O-Sc-O 92.28(1)° observed in the compound SCBO3.4 These distances and angles are consistent with the chemical nonequivalence of the two Sc sites. The origin of this nonequivalence is best appreciated by considering the associations between the Sc and Sr environments as depicted in Figure 3. The Ol octahedron shares triangular faces with Sr-centered polyhedra, while the 02 octahedron shares only vertices. Because the symmetry of the O octahedra is S&, each of the six triangular faces of the Ol polyhedron (related by the improper — = (4) Keszler, D. A.; Sun, H. Acta Crystallogr., Sect. C 1988, 49,1505. Figure 3. Drawing of a portion of the structure of Sr3Sc(B03)3 emphasizing linkages between the Sr- and Sc-centered polyhedra. rotation axis) is shared by a Sr-centered polyhedron, and each vertex of the 02 polyhedron is shared by two Srcentered environments. This results in placement of a distorted octahedron of Sr atoms about the coordination environment of atom Scl and a distorted icosahedron about Sc2. The trigonal compression of the Ol octahedron results from the decrease in its edge lengths from face sharing. The trigonal height of the 02 octahedron is determined by the span Sr—(03-03)—Sr in conjunction with the metrical and electrostatic requirements of the Sr and Sc atoms; the disposition of atom 03 is largely fixed through its interaction with the B atom to form the triangular planar BO3 group. Sr-0 distances, 2.500(2)—2.857(2) A, are normal with the average length 2.69(12) A comparing well to the value 2.71 A computed from empirically derived radii/’ The O environment about the Sr atom may be described as a highly distorted, capped square antiprism. By sharing vertexes, edges, and faces, each Sr-centered (5) Shannon, R. D. Acta Crystallogr., Sect. A 1976, 32, 751. Structure of Sr^ScfBO.i);i o Figure axis. 4. View Chem. Mater., Vol. 6, No. 11, 1994 o of the structure of SrjSclBO.sh along the c polyhedron associates with 11 others of the same type to form a complete three-dimensional framework. The borate group is regular with the average B—O distance 1.38(1) A comparing well to the 1.379 A value deduced from crystal radii. The packing of the borate groups, however, is unique, affording the pinwheel pattern as seen in the view along the c axis (Figure 4). This contrasts to the more common packings of orthoborate groups that are typically found in layered-type structures related to those of the minerals calcite, dolomite, and huntite. Atoms 01 and 03 occupy 5-coordinate sites that are best described as highly distorted triangular bipyra- 2007 mids; atom 01 binds 3 Sr, 1 Sc, and 1 B (Sc-01—B = 135.0(2)°), while atom 03 binds 4 Sr and 1 B. Atom 02 resides in a distorted tetrahedral site comprised of 2 Sr, 1 Sc, and 1 B (B-02-Sc2 = 114.5(2)°). All of these coordination numbers are greater than the 3-coordination of the O atom in the calcite derivative SCBO3. This feature contributes to the high density of the title compound and its thermodynamic stability with respect to a simple mixture of the phases SrstBOsla and SCBO3. The formula volume of the compound Sr3Sc(B03)3—195.2 A3—is smaller than that computed for the mixture Sr3(B03)2 + ScBOs—198.1 A3—indicating a greater lattice energy and stability for Sr3Sc(BC>3)3 should be observed, even though the Sr atom is 9-coordinate and the Sc atom is 6-coordinate in each compound. We conclude by noting that the results indicate the structure to be highly ordered. In particular, there is no evidence for extensive disorder among the Sr and Sc sites. Acknowledgment. This work was performed with funds provided through Lawrence Livermore National Laboratory (Contract 2143103). D.A.K. thanks the Alfred P. Sloan Foundation for a fellowship. Supplementary Material Available: Listing of complete crystal data and anisotropic displacement coefficients (2 pages). Ordering information is given on any current masthead page.